Enantiomerically enriched, polycrystalline molecular sieves Enantiomerically enriched,...
Embed Size (px)
Transcript of Enantiomerically enriched, polycrystalline molecular sieves Enantiomerically enriched,...
Enantiomerically enriched, polycrystalline molecular sieves Stephen K. Branda, Joel E. Schmidta,b, Michael W. Deemc,d, Frits Daeyaertc,d, Yanhang Mae, Osamu Terasakie,f, Marat Orazova,g, and Mark E. Davisa,1
aChemical Engineering, California Institute of Technology, Pasadena, CA 91125; bDebye Institute for Nanomaterials Science, Utrecht University, 3584 CG Utrecht, The Netherlands; cDepartment of Bioengineering, Rice University, Houston, TX 77005; dDepartment of Physics & Astronomy, Rice University, Houston, TX 77005; eSchool of Physical Science and Technology, ShanghaiTech University, Shanghai 201210, China; fDepartment of Materials & Environmental Chemistry, Stockholm University, Stockholm SE-10691, Sweden; and gChemical Engineering, Stanford University, Stanford, CA 94305
Contributed by Mark E. Davis, April 3, 2017 (sent for review March 21, 2017; reviewed by Avelino Corma and Alexander Katz)
Zeolite and zeolite-like molecular sieves are being used in a large number of applications such as adsorption and catalysis. Achieve- ment of the long-standing goal of creating a chiral, polycrystalline molecular sieve with bulk enantioenrichment would enable these materials to perform enantioselective functions. Here, we report the synthesis of enantiomerically enriched samples of a molecular sieve. Enantiopure organic structure directing agents are designed with the assistance of computational methods and used to synthesize enantioenriched, polycrystalline molecular sieve sam- ples of either enantiomer. Computational results correctly pre- dicted which enantiomer is obtained, and enantiomeric enrichment is proven by high-resolution transmission electron microscopy. The enantioenriched and racemic samples of the molecular sieves are tested as adsorbents and heterogeneous catalysts. The enantioen- riched molecular sieves show enantioselectivity for the ring opening reaction of epoxides and enantioselective adsorption of 2-butanol (the R enantiomer of the molecular sieve shows opposite and approximately equal enantioselectivity compared with the S enan- tiomer of the molecular sieve, whereas the racemic sample of the molecular sieve shows no enantioselectivity).
chirality | zeolite | asymmetric catalysis | chiral adsorption
The synthesis of zeolites and zeolite-like molecular sieves hasbeen accomplished using organic structure-directing agents (OSDAs) (1–4). This synthetic method uses an organic molecule (OSDA) to interact with and influence the assembly pathway of the inorganic components to create a crystalline, organic– inorganic composite material. Upon removal of the OSDA, the microporous void space that is created can be exploited in a variety of applications (i.e., catalysis, separations, ion exchange, and ad- sorption) (5). These microporous, polycrystalline materials are 3D networks of oxide tetrahedra [zeolites contain only silicon and aluminum, whereas zeolite-like molecular sieves can have a broader range of elements (1–5)] that create highly ordered, hydrothermally stable framework structures with pores of sizes less than 2 nm. Molecular sieves provide shape-selective properties and, coupled with the inclusion of catalytic active sites, are capable of in- numerable highly selective chemical reactions. Despite the abun- dance of chirality in nature, the discovery of a zeolite or zeolite-like microporous material with enantioselective properties has remained elusive. Enantioenriched, chiral zeolitic materials are of particular interest for their potential to provide robust, new, enantiospecific, shape-selective catalytic pathways and separation processes (6–13). Several inherently chiral molecular sieves have been synthesized
to date (although the bulk, polycrystalline samples are racemic), including *BEA, CZP, GOO, -ITV, JRY, LTJ, OSO, SFS, and STW [molecular sieve framework types are designated by three- letter codes that define the unique connectivity of the oxide tetra- hedral (14)]. In particular, several studies have reported polymorph A (which possesses a chiral helical pore) enriched *BEA. However, zeolite *BEA is limited in that the material crystallizes as highly faulted intergrowths of a racemic mixture of polymorph A and
polymorph B (achiral). In 1992, Davis and Lobo (15) discussed the concept of synthesizing a chiral *BEAmolecular sieve via the use of a chiral OSDA and reported low enantioenrichment (ee) for both a chemical reaction and an adsorption experiment. Recently, Tong et al. (16) have reported a high-fluoride method of synthesizing polymorph A enriched *BEA using achiral OSDAs (although it is difficult to understand the origin of the proposed enantioenrich- ment) and reported low ee’s from a chemical reaction. Other au- thors have reported samples enriched in polymorph A with similar ambiguity in enantioenrichment (17–20). These studies suggest the viability of synthesizing an enantioenriched, chiral molecular sieve. However, the inherent difficulty in controlling the synthesis of polymorphic domains, and the enantiomeric domains of only polymorph A in *BEA, has made it very problematic to conclusively prove that a bulk sample of a molecular sieve does in fact have an enantiomerically enriched framework content. Davis and Lobo (15) discussed this issue and suggested that a preferred approach would be to design syntheses that target chiral molecular sieve structures where individual crystals are single enantiomorphs (microporous analogs to quartz). The STW framework is an example of this type of molecular sieve; recent evidence shows that each individual crystal is a single enantiomorph (i.e., there are no polymorph or opposite enantiomeric domains within a single crystal) (21). A molecular sieve with the STW framework was initially syn-
thesized as a germanosilicate (denoted SU-32) in 2008 (22) and then as a hydrothermally stable pure-silica material in 2012 (23).
Zeolites and zeolite-like molecular sieves are used as adsor- bents and heterogeneous catalysts to prepare a wide variety of products ranging from gasoline to monomers for polymers such as polyethylene terephthalate, which is used in plastic bottles. Pharmaceuticals, pesticides, fragrances, and components in food can contain chiral centers. Here, we prepare enantioen- riched polycrystalline samples of a molecular sieve and show that this type of porous material can function as an adsorbent to separate chiral molecules and as a heterogeneous catalyst to perform chiral reactions. This initial demonstration proves that bulk, enantioenriched chiral zeolites and zeolite-like molecular sieves can be synthesized and that this type of solid can be used to prepare chiral, small molecules.
Author contributions: S.K.B., J.E.S., M.W.D., F.D., Y.M., O.T., M.O., and M.E.D. designed research; S.K.B., J.E.S., Y.M., and M.O. performed research; S.K.B., J.E.S., M.W.D., Y.M., O.T., M.O., and M.E.D. analyzed data; S.K.B., J.E.S., and M.E.D. wrote the paper; and M.W.D. and F.D. performed computational work.
Reviewers: A.C., Instituto de Tecnología Química (UPV-CSIC); and A.K., University of California, Berkeley.
The authors declare no conflict of interest.
Freely available online through the PNAS open access option. 1To whom correspondence should be addressed. Email: email@example.com.
This article contains supporting information online at www.pnas.org/lookup/suppl/doi:10. 1073/pnas.1704638114/-/DCSupplemental.
www.pnas.org/cgi/doi/10.1073/pnas.1704638114 PNAS Early Edition | 1 of 6
http://crossmark.crossref.org/dialog/?doi=10.1073/pnas.1704638114&domain=pdf&date_stamp=2017-04-26 mailto:firstname.lastname@example.org http://www.pnas.org/lookup/suppl/doi:10.1073/pnas.1704638114/-/DCSupplemental http://www.pnas.org/lookup/suppl/doi:10.1073/pnas.1704638114/-/DCSupplemental www.pnas.org/cgi/doi/10.1073/pnas.1704638114
The STW structure contains 10-membered rings (MRs, the number of oxygen or tetrahedral atoms that make up the ring) that form chiral helical pores (22). Past synthesis protocols that used achiral OSDAs resulted in bulk, polycrystalline samples that were racemic mixtures of the two structural enantiomers. STW, therefore, provides a good model for designing the syn- thesis of bulk, polycrystalline samples of either the “R” or “S” enantiomers of the framework. Here, we use computational methods to aid in our design of chiral OSDAs for the synthesis of enantioenriched STW and show that a bulk sample of a poly- crystalline, molecular sieve can be synthesized with significant enantiomeric enrichment. Our design (shown in Fig. 1) provides for the synthesis of either the R or the S enantiomers of STW, thus yielding materials that enable appropriate control experi- ments when elucidating structures and functions.
Results and Discussion Directed Computational Design of a Chiral OSDA for STW. Schmidt et al. (24) reported on the synthesis of STW using a computa- tionally predicted OSDA. This work demonstrated the feasibility of a priori predicting chemically synthesizable monoquaternary, imidazolium OSDAs to create a specified, fluoride-mediated, pure-silica framework. Additionally, STW has been reported to form using diquaternary imidazolium-based OSDAs that are of sufficient size to conform to 10MR channel structure, implying more rigid, chiral analogs may be included in the framework of STW, and may potentially impart structural chirality (24–28). Here, we implemented the previously published computational method implemented by Schmidt et al. (24) and Pophale et al. (29) and used the molecular design constraints suggested by Davis and Lobo (15).